#------------------------------------------------------------------------------
#$Date: 2020-10-06 12:29:41 +0300 (Tue, 06 Oct 2020) $
#$Revision: 257630 $
#$URL: file:///home/coder/svn-repositories/cod/cif/1/55/87/1558790.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_1558790
loop_
_publ_author_name
'Zhang, Zhong'
'Wang, Yue-Lin'
'Liu, Yan'
'Huang, Sheng-Li'
'Yang, Guo-Yu'
_publ_section_title
;
 Three ring-shaped Zr(iv)-substituted silicotungstates: syntheses,
 structures and their properties.
;
_journal_issue                   35
_journal_name_full               Nanoscale
_journal_page_first              18333
_journal_page_last               18341
_journal_paper_doi               10.1039/d0nr02945a
_journal_volume                  12
_journal_year                    2020
_chemical_formula_sum            'B6 H118 Na8 O216 Si4 W40 Zr8'
_chemical_formula_weight         12019.84
_space_group_crystal_system      orthorhombic
_space_group_IT_number           63
_space_group_name_Hall           '-C 2c 2'
_space_group_name_H-M_alt        'C m c m'
_audit_creation_method           SHELXL-2018/3
_audit_update_record
;
2020-07-23 deposited with the CCDC.	2020-08-03 downloaded from the CCDC.
;
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   44.1472(14)
_cell_length_b                   12.5213(5)
_cell_length_c                   41.9116(14)
_cell_measurement_reflns_used    8137
_cell_measurement_temperature    293(2)
_cell_measurement_theta_max      29.5745
_cell_measurement_theta_min      2.8822
_cell_volume                     23167.9(14)
_computing_cell_refinement       'Bruker FRAMBO'
_computing_data_collection       'Bruker FRAMBO'
_computing_data_reduction        'Bruker SAINT'
_computing_molecular_graphics    'Bruker SHELXTL'
_computing_publication_material  'Bruker SHELXTL'
_computing_structure_refinement  'SHELXL-2018/3 (Sheldrick, 2018)'
_computing_structure_solution    'Bruker SHELXTL'
_diffrn_ambient_temperature      293(2)
_diffrn_measured_fraction_theta_full 0.997
_diffrn_measured_fraction_theta_max 0.997
_diffrn_measurement_device_type  'multiwire proportional'
_diffrn_measurement_method       'phi and omega scans'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0524
_diffrn_reflns_av_unetI/netI     0.0607
_diffrn_reflns_Laue_measured_fraction_full 0.997
_diffrn_reflns_Laue_measured_fraction_max 0.997
_diffrn_reflns_limit_h_max       41
_diffrn_reflns_limit_h_min       -52
_diffrn_reflns_limit_k_max       9
_diffrn_reflns_limit_k_min       -14
_diffrn_reflns_limit_l_max       46
_diffrn_reflns_limit_l_min       -49
_diffrn_reflns_number            34875
_diffrn_reflns_point_group_measured_fraction_full 0.997
_diffrn_reflns_point_group_measured_fraction_max 0.997
_diffrn_reflns_theta_full        25.010
_diffrn_reflns_theta_max         25.010
_diffrn_reflns_theta_min         2.888
_diffrn_source                   'sealed tube'
_exptl_absorpt_coefficient_mu    20.253
_exptl_absorpt_correction_T_max  1.00000
_exptl_absorpt_correction_T_min  0.61603
_exptl_absorpt_correction_type   multi-scan
_exptl_crystal_colour            colorless
_exptl_crystal_density_diffrn    3.446
_exptl_crystal_description       block
_exptl_crystal_F_000             21200
_exptl_crystal_size_max          0.180
_exptl_crystal_size_mid          0.140
_exptl_crystal_size_min          0.080
_refine_diff_density_max         3.642
_refine_diff_density_min         -3.318
_refine_diff_density_rms         0.576
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.091
_refine_ls_hydrogen_treatment    undef
_refine_ls_matrix_type           full
_refine_ls_number_parameters     656
_refine_ls_number_reflns         10487
_refine_ls_number_restraints     1350
_refine_ls_restrained_S_all      1.030
_refine_ls_R_factor_all          0.0871
_refine_ls_R_factor_gt           0.0670
_refine_ls_shift/su_max          0.001
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'w=1/[σ²(Fo²)+(0.0524P)²+6084.9272P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.1548
_refine_ls_wR_factor_ref         0.1668
_reflns_Friedel_coverage         0.000
_reflns_number_gt                7956
_reflns_number_total             10487
_reflns_threshold_expression     'I > 2σ(I)'
_cod_data_source_file            d0nr02945a2.cif
_cod_data_source_block           3100_sqd
_cod_depositor_comments
'Adding full bibliography for 1558789--1558791.cif.'
_cod_database_code               1558790
_shelx_shelxl_version_number     2018/3
_shelx_space_group_comment
;
The symmetry employed for this shelxl refinement is uniquely defined
by the following loop, which should always be used as a source of
symmetry information in preference to the above space-group names.
They are only intended as comments.
;
_shelx_estimated_absorpt_t_min   0.121
_shelx_estimated_absorpt_t_max   0.294
loop_
_space_group_symop_operation_xyz
'x, y, z'
'-x, -y, z+1/2'
'-x, y, -z+1/2'
'x, -y, -z'
'x+1/2, y+1/2, z'
'-x+1/2, -y+1/2, z+1/2'
'-x+1/2, y+1/2, -z+1/2'
'x+1/2, -y+1/2, -z'
'-x, -y, -z'
'x, y, -z-1/2'
'x, -y, z-1/2'
'-x, y, z'
'-x+1/2, -y+1/2, -z'
'x+1/2, y+1/2, -z-1/2'
'x+1/2, -y+1/2, z-1/2'
'-x+1/2, y+1/2, z'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_site_symmetry_order
_atom_site_calc_flag
_atom_site_refinement_flags_posn
_atom_site_refinement_flags_adp
_atom_site_refinement_flags_occupancy
_atom_site_disorder_assembly
_atom_site_disorder_group
Zr1 Zr 0.12172(5) 0.23519(18) 0.28995(5) 0.0149(5) Uani 1 1 d . . . . .
Zr2 Zr 0.03791(4) 0.35940(17) 0.38274(5) 0.0116(4) Uani 1 1 d . . . . .
Si1 Si 0.12536(13) 0.2980(5) 0.38166(13) 0.0073(11) Uani 1 1 d . . . . .
W1 W 0.07725(2) 0.10860(8) 0.34902(2) 0.0143(2) Uani 1 1 d . . . . .
W2 W 0.09382(2) 0.53582(7) 0.41147(2) 0.0143(2) Uani 1 1 d . . . . .
W3 W 0.09127(2) 0.48632(8) 0.33259(2) 0.0134(2) Uani 1 1 d . . . . .
W4 W 0.17787(2) 0.49302(8) 0.41001(2) 0.0192(2) Uani 1 1 d . . . . .
W5 W 0.15191(2) 0.05867(8) 0.34692(2) 0.0179(2) Uani 1 1 d . . . . .
W6 W 0.17324(2) 0.43976(9) 0.33114(2) 0.0202(2) Uani 1 1 d . . . . .
W7 W 0.20456(2) 0.26078(9) 0.38119(3) 0.0227(2) Uani 1 1 d . . . . .
W8 W 0.08039(2) 0.15712(8) 0.43527(2) 0.0161(2) Uani 1 1 d . . . . .
W9 W 0.12997(2) 0.33684(8) 0.46512(2) 0.0178(2) Uani 1 1 d . . . . .
W10 W 0.15572(2) 0.10441(8) 0.43511(2) 0.0181(2) Uani 1 1 d . . . . .
B1 B 0.1106(12) 0.001(5) 0.250000 0.043(12) Uani 1 2 d S TU P . .
B2 B 0.000000 0.591(5) 0.3773(19) 0.060(19) Uani 1 2 d S T P . .
B3 B 0.000000 0.296(5) 0.3178(14) 0.048(12) Uani 1 2 d S TU P . .
Na1 Na 0.1417(3) 0.2823(10) 0.5522(3) 0.039(3) Uani 1 1 d . . . . .
Na2 Na 0.2250(3) 0.6601(11) 0.4760(3) 0.042(3) Uani 1 1 d . . . . .
O1 O 0.1531(6) 0.262(2) 0.250000 0.027(3) Uani 1 2 d S TU P . .
O2 O 0.0944(6) 0.295(2) 0.250000 0.030(3) Uani 1 2 d S TU P . .
O3 O 0.1165(6) 0.110(2) 0.250000 0.029(3) Uani 1 2 d S TU P . .
O4 O 0.1060(6) -0.056(2) 0.2226(5) 0.054(5) Uani 1 1 d . U . . .
O5 O 0.000000 0.313(2) 0.4111(6) 0.024(3) Uani 1 2 d S TU P . .
O6 O 0.000000 0.484(2) 0.3809(6) 0.025(3) Uani 1 2 d S TU P . .
O7 O -0.0263(4) 0.6505(16) 0.3723(6) 0.041(4) Uani 1 1 d . U . . .
O8 O 0.000000 0.310(2) 0.3503(6) 0.027(3) Uani 1 2 d S TU P . .
O9 O 0.0258(5) 0.2889(17) 0.2983(5) 0.040(3) Uani 1 1 d . U . . .
O10 O 0.1047(4) 0.4395(14) 0.4451(4) 0.0203(18) Uani 1 1 d . U . . .
O11 O 0.1573(4) 0.3308(14) 0.3099(4) 0.0232(18) Uani 1 1 d . U . . .
O12 O 0.1125(4) 0.0028(14) 0.3470(4) 0.021(2) Uani 1 1 d . U . . .
O13 O 0.0979(4) 0.3648(14) 0.3102(4) 0.0223(19) Uani 1 1 d . U . . .
O14 O 0.0521(4) 0.4518(14) 0.3444(4) 0.0212(19) Uani 1 1 d . U . . .
O15 O 0.1849(4) 0.1560(14) 0.3560(4) 0.0214(19) Uani 1 1 d . U . . .
O16 O 0.1238(3) 0.2455(13) 0.4175(4) 0.0183(17) Uani 1 1 d . U . . .
O17 O 0.1589(4) 0.3539(13) 0.3779(4) 0.0202(17) Uani 1 1 d . U . . .
O18 O 0.1159(4) 0.0660(13) 0.4470(4) 0.020(2) Uani 1 1 d . U . . .
O19 O 0.1860(4) 0.5349(14) 0.3681(4) 0.023(2) Uani 1 1 d . U . . .
O20 O 0.0857(4) 0.1434(14) 0.3070(4) 0.023(2) Uani 1 1 d . U . . .
O21 O 0.0824(4) 0.0878(13) 0.3961(4) 0.0198(19) Uani 1 1 d . U . . .
O22 O 0.0847(4) 0.5814(14) 0.3034(4) 0.023(3) Uani 1 1 d . U . . .
O23 O 0.1360(4) 0.5109(14) 0.3356(4) 0.0213(19) Uani 1 1 d . U . . .
O24 O 0.1726(4) -0.0561(14) 0.3399(4) 0.023(3) Uani 1 1 d . U . . .
O25 O 0.0997(3) 0.3910(13) 0.3786(4) 0.0178(17) Uani 1 1 d . U . . .
O26 O 0.2098(4) 0.3855(14) 0.4066(4) 0.023(2) Uani 1 1 d . U . . .
O27 O 0.1628(4) 0.4062(14) 0.4455(4) 0.0225(17) Uani 1 1 d . U . . .
O28 O 0.1387(4) 0.5488(14) 0.4078(4) 0.0206(18) Uani 1 1 d . U . . .
O29 O 0.1964(4) 0.5916(15) 0.4312(4) 0.026(2) Uani 1 1 d . U . . .
O30 O 0.1211(4) 0.2039(13) 0.3556(4) 0.0185(17) Uani 1 1 d . U . . .
O31 O 0.1513(4) 0.0480(14) 0.3943(4) 0.0197(18) Uani 1 1 d . U . . .
O32 O 0.0949(4) 0.2453(13) 0.4708(4) 0.0197(19) Uani 1 1 d . U . . .
O33 O 0.0488(4) 0.0152(14) 0.3440(4) 0.022(3) Uani 1 1 d . U . . .
O34 O 0.0551(4) 0.4830(13) 0.4122(4) 0.0200(19) Uani 1 1 d . U . . .
O35 O 0.1911(4) 0.5150(15) 0.3017(4) 0.029(3) Uani 1 1 d . U . . .
O36 O 0.2076(4) 0.3508(14) 0.3447(4) 0.024(2) Uani 1 1 d . U . . .
O37 O 0.1876(4) 0.1922(14) 0.4180(4) 0.0215(19) Uani 1 1 d . U . . .
O38 O 0.0890(4) 0.6514(14) 0.4333(4) 0.022(2) Uani 1 1 d . U . . .
O39 O 0.1777(4) 0.0117(14) 0.4535(4) 0.024(3) Uani 1 1 d . U . . .
O40 O 0.0543(4) 0.0831(14) 0.4557(4) 0.024(3) Uani 1 1 d . U . . .
O41 O 0.1338(4) 0.3790(15) 0.5039(4) 0.025(2) Uani 1 1 d . U . . .
O42 O 0.2410(4) 0.2124(15) 0.3818(4) 0.030(4) Uani 1 1 d . U . . .
O43 O 0.1556(4) 0.2133(14) 0.4683(4) 0.0220(19) Uani 1 1 d . U . . .
O44 O 0.0580(3) 0.2654(13) 0.4201(4) 0.0195(19) Uani 1 1 d . U . . .
O45 O 0.0561(4) 0.2283(14) 0.3579(4) 0.0201(18) Uani 1 1 d . U . . .
O46 O 0.0914(4) 0.5913(14) 0.3700(4) 0.019(2) Uani 1 1 d . U . . .
O47 O 0.1496(4) 0.1099(14) 0.3064(4) 0.022(2) Uani 1 1 d . U . . .
O1W O 0.1100(4) 0.1411(15) 0.5297(5) 0.034(3) Uani 1 1 d . U . . .
O2W O 0.1869(4) 0.2064(15) 0.5251(4) 0.031(3) Uani 1 1 d . U . . .
O3W O 0.1488(6) 0.1883(19) 0.5983(6) 0.056(5) Uani 1 1 d . U . . .
O4W O 0.2590(6) 0.525(2) 0.4497(6) 0.060(5) Uani 1 1 d . U . . .
O5W O 0.1976(6) 0.500000 0.500000 0.031(3) Uani 1 2 d S TU P . .
O6W O 0.2351(5) 0.7003(18) 0.5320(5) 0.043(4) Uani 1 1 d . U . . .
O7W O 0.9631(7) 0.830(3) 0.3584(7) 0.079(7) Uani 1 1 d . U . . .
O8W O 0.9273(7) 0.863(3) 0.4035(8) 0.085(7) Uani 1 1 d . U . . .
O9W O 0.1087(7) 0.210(2) 0.6377(7) 0.073(7) Uani 1 1 d . U . . .
O10W O 0.000000 0.529(2) 0.3060(6) 0.033(3) Uani 1 2 d S TU P . .
O11W O 1.000000 0.431(4) 0.250000 0.054(13) Uani 1 4 d S T P . .
O12W O 0.000000 0.169(4) 0.250000 0.043(5) Uani 1 4 d S TU P . .
O13W O 0.0467(6) 0.124(2) 0.250000 0.038(3) Uani 1 2 d S TU P . .
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
B B 0.0013 0.0007 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Si Si 0.0817 0.0704 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Zr Zr -2.9673 0.5597 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
W W -0.8490 6.8722 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Na Na 0.0362 0.0249 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
O20 Zr1 O47 85.6(7) . . ?
O20 Zr1 O13 84.6(7) . . ?
O47 Zr1 O13 137.0(6) . . ?
O20 Zr1 O11 137.0(7) . . ?
O47 Zr1 O11 82.0(7) . . ?
O13 Zr1 O11 77.3(6) . . ?
O20 Zr1 O2 91.7(8) . . ?
O47 Zr1 O2 145.5(8) . . ?
O13 Zr1 O2 76.7(7) . . ?
O11 Zr1 O2 120.6(9) . . ?
O20 Zr1 O1 145.5(8) . . ?
O47 Zr1 O1 89.7(8) . . ?
O13 Zr1 O1 120.2(8) . . ?
O11 Zr1 O1 75.6(7) . . ?
O2 Zr1 O1 73.3(8) . . ?
O20 Zr1 O3 78.3(7) . . ?
O47 Zr1 O3 77.9(7) . . ?
O13 Zr1 O3 139.9(8) . . ?
O11 Zr1 O3 137.4(8) . . ?
O2 Zr1 O3 67.9(8) . . ?
O1 Zr1 O3 67.2(8) . . ?
O20 Zr1 Zr1 110.0(5) . 10_556 ?
O47 Zr1 Zr1 109.1(5) . 10_556 ?
O13 Zr1 Zr1 113.6(5) . 10_556 ?
O11 Zr1 Zr1 113.0(5) . 10_556 ?
O2 Zr1 Zr1 40.3(5) . 10_556 ?
O1 Zr1 Zr1 40.4(5) . 10_556 ?
O3 Zr1 Zr1 43.5(5) . 10_556 ?
O14 Zr2 O45 86.4(7) . . ?
O14 Zr2 O34 86.3(6) . . ?
O45 Zr2 O34 136.1(6) . . ?
O14 Zr2 O5 145.1(7) . . ?
O45 Zr2 O5 111.2(8) . . ?
O34 Zr2 O5 99.0(8) . . ?
O14 Zr2 O44 138.1(6) . . ?
O45 Zr2 O44 77.0(6) . . ?
O34 Zr2 O44 80.1(6) . . ?
O5 Zr2 O44 76.5(7) . . ?
O14 Zr2 O8 84.8(8) . . ?
O45 Zr2 O8 76.8(7) . . ?
O34 Zr2 O8 145.1(7) . . ?
O5 Zr2 O8 71.2(8) . . ?
O44 Zr2 O8 126.8(8) . . ?
O14 Zr2 O6 79.2(7) . . ?
O45 Zr2 O6 142.7(7) . . ?
O34 Zr2 O6 77.5(7) . . ?
O5 Zr2 O6 68.5(8) . . ?
O44 Zr2 O6 134.4(8) . . ?
O8 Zr2 O6 67.8(8) . . ?
O14 Zr2 Zr2 107.5(4) . 12 ?
O45 Zr2 Zr2 112.5(4) . 12 ?
O34 Zr2 Zr2 111.0(4) . 12 ?
O5 Zr2 Zr2 38.4(5) . 12 ?
O44 Zr2 Zr2 114.4(4) . 12 ?
O8 Zr2 Zr2 41.7(5) . 12 ?
O6 Zr2 Zr2 43.1(5) . 12 ?
O30 Si1 O16 108.8(9) . . ?
O30 Si1 O25 112.7(9) . . ?
O16 Si1 O25 109.1(8) . . ?
O30 Si1 O17 110.4(9) . . ?
O16 Si1 O17 107.3(8) . . ?
O25 Si1 O17 108.3(9) . . ?
O33 W1 O45 102.2(8) . . ?
O33 W1 O20 100.9(8) . . ?
O45 W1 O20 96.0(7) . . ?
O33 W1 O21 96.5(7) . . ?
O45 W1 O21 87.8(7) . . ?
O20 W1 O21 160.9(7) . . ?
O33 W1 O12 96.3(7) . . ?
O45 W1 O12 160.0(7) . . ?
O20 W1 O12 87.8(7) . . ?
O21 W1 O12 82.6(7) . . ?
O33 W1 O30 168.8(7) . . ?
O45 W1 O30 88.8(7) . . ?
O20 W1 O30 79.8(7) . . ?
O21 W1 O30 81.6(6) . . ?
O12 W1 O30 72.5(6) . . ?
O38 W2 O34 100.4(8) . . ?
O38 W2 O46 99.9(8) . . ?
O34 W2 O46 95.5(7) . . ?
O38 W2 O10 99.7(8) . . ?
O34 W2 O10 89.8(7) . . ?
O46 W2 O10 158.4(7) . . ?
O38 W2 O28 95.4(7) . . ?
O34 W2 O28 163.2(7) . . ?
O46 W2 O28 87.4(7) . . ?
O10 W2 O28 81.9(7) . . ?
O38 W2 O25 175.0(7) . . ?
O34 W2 O25 80.2(6) . . ?
O46 W2 O25 75.1(6) . . ?
O10 W2 O25 85.2(6) . . ?
O28 W2 O25 84.6(6) . . ?
O38 W2 Na1 44.7(6) . 4_566 ?
O34 W2 Na1 143.2(6) . 4_566 ?
O46 W2 Na1 101.4(5) . 4_566 ?
O10 W2 Na1 86.4(5) . 4_566 ?
O28 W2 Na1 51.2(5) . 4_566 ?
O25 W2 Na1 135.7(4) . 4_566 ?
O22 W3 O13 103.7(8) . . ?
O22 W3 O14 101.1(8) . . ?
O13 W3 O14 95.4(7) . . ?
O22 W3 O23 96.0(7) . . ?
O13 W3 O23 90.2(7) . . ?
O14 W3 O23 160.2(7) . . ?
O22 W3 O46 95.8(7) . . ?
O13 W3 O46 159.4(7) . . ?
O14 W3 O46 87.0(7) . . ?
O23 W3 O46 81.4(7) . . ?
O22 W3 O25 167.7(7) . . ?
O13 W3 O25 88.5(7) . . ?
O14 W3 O25 78.8(6) . . ?
O23 W3 O25 82.4(6) . . ?
O46 W3 O25 71.9(6) . . ?
O29 W4 O19 101.1(8) . . ?
O29 W4 O28 101.3(8) . . ?
O19 W4 O28 91.5(7) . . ?
O29 W4 O27 99.6(8) . . ?
O19 W4 O27 159.3(7) . . ?
O28 W4 O27 86.1(7) . . ?
O29 W4 O26 100.9(8) . . ?
O19 W4 O26 89.2(7) . . ?
O28 W4 O26 157.2(7) . . ?
O27 W4 O26 85.2(7) . . ?
O29 W4 O17 172.3(7) . . ?
O19 W4 O17 74.8(7) . . ?
O28 W4 O17 85.4(6) . . ?
O27 W4 O17 84.5(6) . . ?
O26 W4 O17 72.9(6) . . ?
O29 W4 Na1 54.9(6) . 4_566 ?
O19 W4 Na1 106.3(6) . 4_566 ?
O28 W4 Na1 47.1(5) . 4_566 ?
O27 W4 Na1 87.1(5) . 4_566 ?
O26 W4 Na1 152.8(5) . 4_566 ?
O17 W4 Na1 132.2(4) . 4_566 ?
O24 W5 O47 99.4(8) . . ?
O24 W5 O12 100.4(8) . . ?
O47 W5 O12 94.6(7) . . ?
O24 W5 O15 99.1(8) . . ?
O47 W5 O15 90.2(7) . . ?
O12 W5 O15 158.8(7) . . ?
O24 W5 O31 97.0(8) . . ?
O47 W5 O31 162.7(7) . . ?
O12 W5 O31 87.8(7) . . ?
O15 W5 O31 81.8(7) . . ?
O24 W5 O30 175.7(7) . . ?
O47 W5 O30 80.5(7) . . ?
O12 W5 O30 75.3(7) . . ?
O15 W5 O30 85.2(6) . . ?
O31 W5 O30 83.6(6) . . ?
O35 W6 O11 103.9(8) . . ?
O35 W6 O23 102.1(8) . . ?
O11 W6 O23 93.9(7) . . ?
O35 W6 O36 99.4(8) . . ?
O11 W6 O36 90.8(8) . . ?
O23 W6 O36 156.2(7) . . ?
O35 W6 O19 95.6(8) . . ?
O11 W6 O19 160.4(7) . . ?
O23 W6 O19 83.7(7) . . ?
O36 W6 O19 84.2(7) . . ?
O35 W6 O17 166.4(7) . . ?
O11 W6 O17 87.6(7) . . ?
O23 W6 O17 84.1(6) . . ?
O36 W6 O17 72.8(6) . . ?
O19 W6 O17 72.8(6) . . ?
O42 W7 O15 101.1(8) . . ?
O42 W7 O36 98.9(8) . . ?
O15 W7 O36 89.6(7) . . ?
O42 W7 O37 101.3(8) . . ?
O15 W7 O37 87.7(7) . . ?
O36 W7 O37 159.7(7) . . ?
O42 W7 O26 99.7(8) . . ?
O15 W7 O26 159.3(7) . . ?
O36 W7 O26 87.5(7) . . ?
O37 W7 O26 87.9(7) . . ?
O42 W7 O17 170.2(8) . . ?
O15 W7 O17 85.3(6) . . ?
O36 W7 O17 73.5(6) . . ?
O37 W7 O17 86.2(6) . . ?
O26 W7 O17 74.2(6) . . ?
O40 W8 O44 102.4(8) . . ?
O40 W8 O21 102.8(8) . . ?
O44 W8 O21 93.7(7) . . ?
O40 W8 O32 98.4(8) . . ?
O44 W8 O32 91.4(7) . . ?
O21 W8 O32 156.6(7) . . ?
O40 W8 O18 95.5(8) . . ?
O44 W8 O18 161.8(7) . . ?
O21 W8 O18 85.1(7) . . ?
O32 W8 O18 83.0(7) . . ?
O40 W8 O16 166.0(7) . . ?
O44 W8 O16 88.9(6) . . ?
O21 W8 O16 84.4(6) . . ?
O32 W8 O16 72.9(6) . . ?
O18 W8 O16 72.9(6) . . ?
O41 W9 O10 105.5(8) . . ?
O41 W9 O43 97.2(8) . . ?
O10 W9 O43 157.3(7) . . ?
O41 W9 O27 101.3(8) . . ?
O10 W9 O27 87.0(7) . . ?
O43 W9 O27 87.0(7) . . ?
O41 W9 O32 98.3(7) . . ?
O10 W9 O32 89.2(7) . . ?
O43 W9 O32 89.2(7) . . ?
O27 W9 O32 160.4(7) . . ?
O41 W9 O16 168.2(7) . . ?
O10 W9 O16 83.4(6) . . ?
O43 W9 O16 74.4(6) . . ?
O27 W9 O16 86.7(6) . . ?
O32 W9 O16 73.7(6) . . ?
O39 W10 O31 102.5(8) . . ?
O39 W10 O18 103.7(8) . . ?
O31 W10 O18 92.8(7) . . ?
O39 W10 O37 98.2(8) . . ?
O31 W10 O37 87.2(7) . . ?
O18 W10 O37 157.5(7) . . ?
O39 W10 O43 99.0(8) . . ?
O31 W10 O43 157.2(7) . . ?
O18 W10 O43 89.3(7) . . ?
O37 W10 O43 82.3(7) . . ?
O39 W10 O16 171.0(7) . . ?
O31 W10 O16 86.3(6) . . ?
O18 W10 O16 73.7(6) . . ?
O37 W10 O16 83.9(6) . . ?
O43 W10 O16 72.5(6) . . ?
O3 B1 O4 123(2) . 10_556 ?
O3 B1 O4 123(2) . . ?
O4 B1 O4 115(5) 10_556 . ?
O6 B2 O7 123(2) . . ?
O6 B2 O7 123(2) . 12 ?
O7 B2 O7 113(5) . 12 ?
O9 B3 O9 108(4) . 12 ?
O9 B3 O8 126(2) . . ?
O9 B3 O8 126(2) 12 . ?
O3W Na1 O41 179.2(11) . . ?
O3W Na1 O1W 91.8(9) . . ?
O41 Na1 O1W 87.5(7) . . ?
O3W Na1 O2W 94.6(8) . . ?
O41 Na1 O2W 85.7(7) . . ?
O1W Na1 O2W 90.4(7) . . ?
O3W Na1 O38 95.2(8) . 4_566 ?
O41 Na1 O38 84.5(7) . 4_566 ?
O1W Na1 O38 78.8(7) . 4_566 ?
O2W Na1 O38 165.6(8) . 4_566 ?
O3W Na1 O28 83.4(8) . 4_566 ?
O41 Na1 O28 97.0(7) . 4_566 ?
O1W Na1 O28 141.1(7) . 4_566 ?
O2W Na1 O28 128.5(7) . 4_566 ?
O38 Na1 O28 63.4(6) 4_566 4_566 ?
O3W Na1 O29 88.0(8) . 4_566 ?
O41 Na1 O29 92.8(7) . 4_566 ?
O1W Na1 O29 160.3(7) . 4_566 ?
O2W Na1 O29 70.0(6) . 4_566 ?
O38 Na1 O29 120.9(7) 4_566 4_566 ?
O28 Na1 O29 58.5(5) 4_566 4_566 ?
O3W Na1 W2 92.9(7) . 4_566 ?
O41 Na1 W2 87.1(5) . 4_566 ?
O1W Na1 W2 107.2(6) . 4_566 ?
O2W Na1 W2 160.7(7) . 4_566 ?
O38 Na1 W2 28.5(4) 4_566 4_566 ?
O28 Na1 W2 35.1(4) 4_566 4_566 ?
O29 Na1 W2 92.5(5) 4_566 4_566 ?
O3W Na1 W4 88.3(7) . 4_566 ?
O41 Na1 W4 92.4(6) . 4_566 ?
O1W Na1 W4 171.3(6) . 4_566 ?
O2W Na1 W4 98.3(6) . 4_566 ?
O38 Na1 W4 92.6(5) 4_566 4_566 ?
O28 Na1 W4 30.4(4) 4_566 4_566 ?
O29 Na1 W4 28.4(4) 4_566 4_566 ?
W2 Na1 W4 64.1(2) 4_566 4_566 ?
O3W Na1 Na2 102.8(8) . 4_566 ?
O41 Na1 Na2 77.8(5) . 4_566 ?
O1W Na1 Na2 123.5(6) . 4_566 ?
O2W Na1 Na2 35.1(5) . 4_566 ?
O38 Na1 Na2 150.2(6) 4_566 4_566 ?
O28 Na1 Na2 95.1(5) 4_566 4_566 ?
O29 Na1 Na2 38.0(4) 4_566 4_566 ?
W2 Na1 Na2 125.7(4) 4_566 4_566 ?
W4 Na1 Na2 64.8(3) 4_566 4_566 ?
O2W Na2 O29 82.2(7) 4_566 . ?
O2W Na2 O6W 90.1(8) 4_566 . ?
O29 Na2 O6W 156.0(8) . . ?
O2W Na2 O6W 90.2(8) 4_566 13_566 ?
O29 Na2 O6W 120.7(8) . 13_566 ?
O6W Na2 O6W 81.8(8) . 13_566 ?
O2W Na2 O4W 152.6(9) 4_566 . ?
O29 Na2 O4W 74.5(8) . . ?
O6W Na2 O4W 116.9(9) . . ?
O6W Na2 O4W 89.5(9) 13_566 . ?
O2W Na2 O5W 103.0(8) 4_566 . ?
O29 Na2 O5W 77.2(6) . . ?
O6W Na2 O5W 82.5(6) . . ?
O6W Na2 O5W 159.4(8) 13_566 . ?
O4W Na2 O5W 85.9(8) . . ?
O2W Na2 Na2 90.2(7) 4_566 13_566 ?
O29 Na2 Na2 159.8(8) . 13_566 ?
O6W Na2 Na2 41.5(5) . 13_566 ?
O6W Na2 Na2 40.2(5) 13_566 13_566 ?
O4W Na2 Na2 106.8(8) . 13_566 ?
O5W Na2 Na2 122.8(6) . 13_566 ?
O2W Na2 Na1 37.0(5) 4_566 4_566 ?
O29 Na2 Na1 48.9(5) . 4_566 ?
O6W Na2 Na1 114.9(7) . 4_566 ?
O6W Na2 Na1 119.3(7) 13_566 4_566 ?
O4W Na2 Na1 123.4(7) . 4_566 ?
O5W Na2 Na1 79.5(6) . 4_566 ?
Na2 Na2 Na1 127.1(6) 13_566 4_566 ?
Zr1 O1 Zr1 99.3(10) 10_556 . ?
Zr1 O2 Zr1 99.4(10) 10_556 . ?
B1 O3 Zr1 133.4(5) . 10_556 ?
B1 O3 Zr1 133.4(5) . . ?
Zr1 O3 Zr1 93.1(10) 10_556 . ?
Zr2 O5 Zr2 103.2(10) 12 . ?
B2 O6 Zr2 133.0(5) . 12 ?
B2 O6 Zr2 133.0(5) . . ?
Zr2 O6 Zr2 93.8(9) 12 . ?
B3 O8 Zr2 129.5(9) . 12 ?
B3 O8 Zr2 129.5(9) . . ?
Zr2 O8 Zr2 96.6(10) 12 . ?
W9 O10 W2 154.0(9) . . ?
W6 O11 Zr1 156.2(10) . . ?
W5 O12 W1 117.7(9) . . ?
W3 O13 Zr1 159.0(9) . . ?
W3 O14 Zr2 128.2(9) . . ?
W7 O15 W5 152.7(9) . . ?
Si1 O16 W9 125.9(9) . . ?
Si1 O16 W8 121.1(8) . . ?
W9 O16 W8 93.3(6) . . ?
Si1 O16 W10 123.7(9) . . ?
W9 O16 W10 91.7(5) . . ?
W8 O16 W10 92.1(6) . . ?
Si1 O17 W7 124.0(9) . . ?
Si1 O17 W6 121.6(9) . . ?
W7 O17 W6 92.7(6) . . ?
Si1 O17 W4 125.4(9) . . ?
W7 O17 W4 91.6(6) . . ?
W6 O17 W4 92.5(6) . . ?
W10 O18 W8 121.3(9) . . ?
W4 O19 W6 119.9(9) . . ?
W1 O20 Zr1 127.4(9) . . ?
W8 O21 W1 143.5(9) . . ?
W6 O23 W3 141.6(10) . . ?
Si1 O25 W2 126.6(9) . . ?
Si1 O25 W3 123.3(9) . . ?
W2 O25 W3 94.3(6) . . ?
W7 O26 W4 121.2(8) . . ?
W9 O27 W4 148.2(9) . . ?
W4 O28 W2 152.3(10) . . ?
W4 O28 Na1 102.5(7) . 4_566 ?
W2 O28 Na1 93.7(7) . 4_566 ?
W4 O29 Na2 154.1(11) . . ?
W4 O29 Na1 96.7(7) . 4_566 ?
Na2 O29 Na1 93.1(7) . 4_566 ?
Si1 O30 W1 123.9(9) . . ?
Si1 O30 W5 127.9(9) . . ?
W1 O30 W5 93.9(6) . . ?
W10 O31 W5 152.9(10) . . ?
W9 O32 W8 120.1(8) . . ?
W2 O34 Zr2 126.0(8) . . ?
W7 O36 W6 120.9(8) . . ?
W7 O37 W10 147.3(9) . . ?
W2 O38 Na1 106.8(8) . 4_566 ?
W9 O41 Na1 131.4(10) . . ?
W9 O43 W10 121.1(8) . . ?
W8 O44 Zr2 154.0(9) . . ?
W1 O45 Zr2 161.5(9) . . ?
W2 O46 W3 118.2(9) . . ?
W5 O47 Zr1 127.0(9) . . ?
Na2 O2W Na1 108.0(8) 4_566 . ?
Na2 O5W Na2 123.2(11) . 4_566 ?
Na2 O6W Na2 98.2(8) . 13_566 ?
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
Zr1 O20 2.089(17) . ?
Zr1 O47 2.109(17) . ?
Zr1 O13 2.112(17) . ?
Zr1 O11 2.146(17) . ?
Zr1 O2 2.195(17) . ?
Zr1 O1 2.197(16) . ?
Zr1 O3 2.307(19) . ?
Zr1 Zr1 3.348(4) 10_556 ?
Zr2 O14 2.076(17) . ?
Zr2 O45 2.104(17) . ?
Zr2 O34 2.119(17) . ?
Zr2 O5 2.135(15) . ?
Zr2 O44 2.150(17) . ?
Zr2 O8 2.242(17) . ?
Zr2 O6 2.292(18) . ?
Zr2 Zr2 3.347(4) 12 ?
Si1 O30 1.618(17) . ?
Si1 O16 1.643(16) . ?
Si1 O25 1.630(17) . ?
Si1 O17 1.646(17) . ?
W1 O33 1.729(16) . ?
W1 O45 1.804(17) . ?
W1 O20 1.852(17) . ?
W1 O21 2.001(16) . ?
W1 O12 2.045(17) . ?
W1 O30 2.292(16) . ?
W2 O38 1.724(17) . ?
W2 O34 1.834(16) . ?
W2 O46 1.873(16) . ?
W2 O10 1.918(17) . ?
W2 O28 1.996(16) . ?
W2 O25 2.292(16) . ?
W2 Na1 3.460(11) 4_566 ?
W3 O22 1.731(17) . ?
W3 O13 1.812(17) . ?
W3 O14 1.851(16) . ?
W3 O23 2.003(16) . ?
W3 O46 2.048(16) . ?
W3 O25 2.298(16) . ?
W4 O29 1.725(18) . ?
W4 O19 1.868(17) . ?
W4 O28 1.866(16) . ?
W4 O27 1.958(17) . ?
W4 O26 1.953(17) . ?
W4 O17 2.356(16) . ?
W4 Na1 3.601(13) 4_566 ?
W5 O24 1.729(17) . ?
W5 O47 1.817(17) . ?
W5 O12 1.875(16) . ?
W5 O15 1.937(17) . ?
W5 O31 1.990(16) . ?
W5 O30 2.300(16) . ?
W6 O35 1.741(17) . ?
W6 O11 1.774(17) . ?
W6 O23 1.879(16) . ?
W6 O36 1.965(17) . ?
W6 O19 2.033(17) . ?
W6 O17 2.322(16) . ?
W7 O42 1.719(18) . ?
W7 O15 1.895(17) . ?
W7 O36 1.906(17) . ?
W7 O37 1.920(17) . ?
W7 O26 1.905(18) . ?
W7 O17 2.333(16) . ?
W8 O40 1.709(16) . ?
W8 O44 1.795(17) . ?
W8 O21 1.861(17) . ?
W8 O32 1.962(16) . ?
W8 O18 2.001(16) . ?
W8 O16 2.333(16) . ?
W9 O41 1.719(17) . ?
W9 O10 1.896(17) . ?
W9 O43 1.922(17) . ?
W9 O27 1.881(17) . ?
W9 O32 1.939(16) . ?
W9 O16 2.315(16) . ?
W10 O39 1.697(16) . ?
W10 O31 1.861(16) . ?
W10 O18 1.889(16) . ?
W10 O37 1.922(17) . ?
W10 O43 1.946(17) . ?
W10 O16 2.378(16) . ?
B1 O3 1.39(6) . ?
B1 O4 1.36(4) 10_556 ?
B1 O4 1.36(4) . ?
B2 O6 1.35(6) . ?
B2 O7 1.39(4) . ?
B2 O7 1.39(4) 12 ?
B3 O9 1.40(4) . ?
B3 O9 1.40(4) 12 ?
B3 O8 1.37(6) . ?
Na1 O3W 2.28(3) . ?
Na1 O41 2.38(2) . ?
Na1 O1W 2.44(2) . ?
Na1 O2W 2.48(2) . ?
Na1 O38 2.54(2) 4_566 ?
Na1 O28 2.70(2) 4_566 ?
Na1 O29 2.97(2) 4_566 ?
Na1 Na2 3.931(16) 4_566 ?
Na2 O2W 2.37(2) 4_566 ?
Na2 O29 2.42(2) . ?
Na2 O6W 2.44(2) . ?
Na2 O6W 2.50(2) 13_566 ?
Na2 O4W 2.51(3) . ?
Na2 O5W 2.549(18) . ?
Na2 Na2 3.74(2) 13_566 ?
